세계 제일의 방대한 재료 데이터베이스

# Fracture Mechanics of Cold-Drawn Copper Bars

요약:

Crack growth occurs in most materials through intense plastic deformation possibly combined with void growth and void coalescence. The region where these processes take place is very small or of about the same size as the crack tip opening displacement.
It is difficult to study these processes experimentally and to model them analytically in any greater detail. For this reason the goal in fracture mechanics is to avoid using detailed information concerning the fracture process zone in a crack growth criterion.

Crack growth occurs in most materials through intense plastic deformation possibly combined with void growth and void coalescence. The region where these processes take place is very small or of about the same size as the crack tip opening displacement. One realizes that it is very difficult to study these processes experimentally and to model them analytically in any greater detail. For this reason the goal in fracture mechanics is to avoid using detailed information concerning the fracture process zone in a crack growth criterion.

Most important is to find one parameter which determines uniquely the state of stress and strain outside the fracture process zone say on a circle of radius ro around the crack tip, Figure 1, and which is related to external boundary conditions, i.e. load and geometry. This parameter will act as a "single parameter" boundary condition for the inner region. If we solve the boundary value problem for the inner region, Figure 1, including the fracture process zone, the state of stress and strain there will be functions of material properties and of the single parameter defining the state at r = ro. The conclusion is then that for each material this parameter uniquely describes the conditions in the fracture process zone and thus may be suitably used in a crack growth criterion. Parameters of this type are under certain conditions the stress intensity factor K and the J-integral.

Figure 1: Boundary conditions for inner region given on circle r with intensity defined in terms of K or J

The failure of a component or a specimen with an elastic plastic material behavior proves to be much more complex than under linear elastic conditions. For the thinner specimens the formation of large plastic zones at the crack tip and crack extension by slow ductile tearing give rise to strongly non-linear load/displacement-curves.

First indications of stable crack growth have been found down to 60 % of the maximum load Fmax. The external load can obviously be increased far beyond this point until the load carrying capacity of the remaining ligament is exceeded and tearing and final catastrophic failure can progress under reducing load. For such a plateau type of behavior it is hard to detect the achievement of maximum load and the corresponding values of crack length and displacement because COD or J determination depend besides geometry and size on machine stiffness and loading rate.

Looking at the crack tip on a microscopic scale reveals even more complex details. Figure 2 summarizes some of our knowledge about the successive stages of the ductile failure process. Starting from a natural sharp defect or an artificial crack of length ao introduced in advance by fatiguing at a low ΔK-level a plastic zone is formed under increasing load F and the crack blunts through local sliding processes. This developing stretch zone, which afterwards can be measured as a definite step on the fracture surface, grows proportional to the load until a critical crack opening displacement δi is reached and a crack advance occurs ahead of the original blunted crack.

The mode of extension at the beginning and further on may be unstable or stable through cleavage or through a continuous process of nucleation, growth and coalescence of voids in the crack tip strain field. This whole process may best be described by plotting a parameter that characterizes the stress/strain-field at the crack tip (J or δ may be chosen for elastic plastic conditions and K or G for linear elastic conditions) against crack growth Δa.

In the lower load regime of crack blunting a linear relationship between J and crack growth Δa is found. But this quasi crack growth is small as compared to that due to tearing at loads near to and at maximum load. The change of slope of the resistance curve is used to define and to measure critical values of δ and J.

Although new concepts are being developed many problems still exist today to describe quantitatively the further crack growth and the final point of tearing instability. Therefore elastic-plastic fracture toughness values are derived for microscopic crack initiation mainly and the safety philosophy is based on critical values δi and Ji for the onset of stable crack growth which appear to represent true material properties.

The simultaneous registration of either the elastic compliance, electrical resistance, acoustic emission, or ultrasonic transmission of the specimen together with load and displacement may be used. The change of either one of these physical properties with crack length allows for the evaluation of critical values of load and displacement.

Figure 2: Successive stages of ductile failure and schematic crack resistance curve

Ductile fracture in metallic alloys usually proceeds by the four stages of:

• void nucleation by failure or interfacial decohesion of second-phase inclusions,
• void growth induced by plastic straining,
• void coalescence by strain localization in the intervoid ligament or by void impingement, and
• propagation of a macroscopic crack by accumulation of void coalescence events, sometimes along shear bands.
Void growth is certainly the most studied of the four stages. Plastic void growth modeling started nearly 30 years ago.

1. Void interaction, which promotes void growth and principally depends on the initial void volume fraction. Void interaction becomes effective mainly during the void coalescence process.

2. Strain hardening, which must be adequately introduced in void growth models or, more precisely, which must be accounted for from proper micromechanical analysis of the enlargement of a void in a strain-hardened material.

3. Void shape, which greatly influences void coalescence. It has been proven that initially spherical voids assume, in the direction of straining, a prelate ellipsoidal shape during growth under low stress triaxiality and an oblate ellipsoidal shape under high stress triaxiality. The initial void shape is imposed the inclusion shape.

4. The presence of the inclusion at which the void nucleates, which, at low stress triaxialities or in cases large shear strains, may hinder contraction of the void. When a void initiates through the fracture of second-phase inclusion, the presence of the inclusions, also affects void growth considerably.

5. Heterogeneity and anisotropy in the distribution voids, which play a key role in the onset of void coalescence or shear localization and explain importance of variations of the ductility of a material when tested in different directions.

6. Elastically driven void growth instabilities, which develop at high stress triaxialities.

7. Inhomogeneous boundary strain rate, which are en countered at crack tips, or local strain gradient, which may develop for very small voids.

8. Plastic anisotropy, which slightly influences void growth.

Most often void growth models have been assessed on ideal materials with a high content of large inclusions created by powder metallurgy. In these materials, quantitative measurements of porosity distribution are possible. However, in industrial alloys, voids frequently remain very small (<10 μm) and porosity is always very low. In steel, void size can be directly measured metallographically by unloading after some extent of straining and by breaking the strained specimen below the brittle-ductile transition temperature. This method preserves void size. In other industrial alloys, direct evaluation of void size in the bulk is less accurate.

Indeed, polishing changes void size. Indirect porosity measurements are, thus, necessary. Porosity distribution and local void dimensions must then be recovered from experimental data, which usually refer to a porosity averaged in a large volume. The determination of the real evolution of porosity distribution is important in order to physically identify the parameters of the void growth models. Prediction of void coalescence by micromechanical criteria requires quantitative modeling of the void interdistance and mutual arrangement.

## 기술 자료 검색

검색할 어구를 입력하십시오:

 검색 범위 본문 키워드 머릿글 요약

Total Materia Extended Range는 수천개 금속 합금의 열처리 조건 및 하중 조건에 대한 파괴 공학 변수 데이터베이스를 포함하고 있습니다. K1C, KC, 균열 성장 및 Paris 법칙 변수와 이에 대응되는 균열 성장 그래프가 제공됩니다.

단조 특성도 참조를 위해 추가되어 있으며 단조 특성을 통해 예상되는 빠진 변수의 추정치도 필요한 곳에는 포함되어 있습니다.

신속 검색에 검색할 재질명을 입력합니다. 원하신다면 국가/규격을 지정하신 후 검색 버튼을 클릭합니다.

결과 리스트에서 재질을 선택하시면, 일련의 규격 사양 소그룹이 나타납니다.

Total Materia 파괴 공학 데이터는 규격 사양서와 무관하므로, 어떠한 소그룹 내의 링크를 클릭하셔도 파괴 공학 데이터를 검토하실 수 있습니다.

데이터는 표로 출력되며, 가능한 곳에는 Paris 곡선(Region II)와 함께 출력되어 있습니다. 데이터 출처에 관한 정확한 참조가 각 데이터에 주어져 있습니다.

Total Materia 데이터베이스를 사용해 보실 수 있는 기회가 있습니다. 저희는 Total Materia 무료 체험을 통해 150,000명 이상의 사용자가 이용하고 있는 커뮤니티로 귀하를 초대합니다.